2. International Journal of Mechanical Engineering Research and Development (IJMERD), ISSN 2248 –9347(Print) ISSN 2228 – 9355(Online), Volume 2, Number 1, January- September (2012)The manufacturing of the natural fiber reinforced composite can broadly be classified asprimary and secondary manufacturing. The primary manufacturing results in a near-netshape of the final product. The various primary manufacturing processes are hand lay-up,pultrusion, filament winding, vacuum bag molding and resin transfer molding. Althoughmost of the composite products are made to a near-net shape, a certain degree of intricacyin the product design necessitates the development of the composite product in parts. Theindependently manufactured parts are then finally assembled to get the final compositeproduct. Machining thus becomes imperative to ascertain the structural integrity ofcomplex composite products. Hole making is one of the important machining operationsto facilitate the assembly operations. Though a number of approaches have been used formaking holes in composite laminates, conventional drilling till date is the most widelyacceptable and frequently practiced machining operation for hole making. Conventionaldrilling however results in damage in the form of delamination, micro cracks, fiber pullout and matrix burning around the hole and may ultimately cause variation in the strengthof the component with a drilled hole.Koenig et al. [6] studied in 1985 the machining of fiber reinforced plastics and concludedthat a high feed rate of drilling will cause a crack around the exit edge of the hole. MillerHocheng and Puw [7] in 1992 presented a study of the chip formation and assess themachinability of two composite materials and concluded that from cutting chips theformer presents a large amount of deformation in chip formation, while the latter tends tofracture. Chambers and Bishop [8] in 1995 investigated the effect of the cuttingparameters on drilling carbon/epoxy and carbon/peek and concluded that the drilling ofcarbon composites is dependent upon the characteristics of the matrix and the helicalPCD drill geometry gave the best overall performance.Lin et al. [9] in 1996, carried out a study on drilling of carbon fiber reinforced compositeat high speed and concluded that an increase of the cutting velocity leads a increasing ofthe drill wear. In this way the fact of increasing the wear of drill causes a rising of thrustforce. Wen-Chou Chen [10] in 1997 studied the variations of cutting forces with orwithout onset delamination during the drilling operations and concluded that thedelamination free drilling processes may be obtained by the proper selections of toolgeometry and drilling parameters. Piquet et al. [11] in 2000 carried out a study of drillingthin carbon/epoxy laminates with two types of drills, a helical drill and a drill of specialgeometry, and concluded that both drills leads a damage at the entrance in the wall andthe exit of the hole, with the exception of special geometry drill which is possible asignificant reduction in the final damage. Enemuoh et al. [12] in 2001, realize that withthe application of the technique of Taguchi and other methods, were possible to achievethe cutting parameters that allowed the absence of damage in the drilling of fiberreinforced plastics.In order to understand the effects of process parameters on the delamination, a largenumber of machining experiments have to be performed and analyzed mathematicalmodels to be built on the same. Modeling of the formation of delaminations is highlycomplex and expensive. Hence, empirical/statistical approaches are widely used over theconventional mathematical models. In this paper, an approach based on the Taguchi 2
3. International Journal of Mechanical Engineering Research and Development (IJMERD), ISSN 2248 –9347(Print) ISSN 2228 – 9355(Online), Volume 2, Number 1, January- September (2012)method is used to determine the desired optimum cutting parameters for minimizedappearance of delaminations in drilled unidirectional hemp fiber reinforced composites.2. EXPERIMENTAL SET-UP AND MACHINING CONDITIONS2.1. HFRP specimen preparationsThe composite materials used in the tests are made with hemp fiber reinforcement. Theresin polyester possessing a modulus of 3.25 GPa and density 1350 kg/m3 was used inpreparing the specimens with hand lay-up process. Required numbers of layers werestacked to give intended thickness and a fiber volume fraction, which was determinedlater to 0.52 using weight loss method.2.2. Machining set-upThe carbide drill bit used in the experiments was of 5mm diameter. Drilling tests wereconducted on CNC machining center supplied by MTAB, India. The laminate compositespecimen was held in a rigid fixture attached to the machine table. The experimental set-up is as shown by the schematic in Fig. 1. Fig. 1. Schematic diagram of experimental set-up.2.3. Design of experimentsThe cutting speed and the feed rate are the two most important parameters thatcharacterize the drilling operation and have been selected for investigation. The feed rateand the speed are the two parameters under investigation in the present study. A L9orthogonal array is selected for the present investigation. The factors and their respectivelevels are shown in Table 1. The treatment of experimental results is based on theanalysis of variance (ANOVA). The analysis of variance of the experimental data for thePeel up delamination and Push down delamination generated during drilling of UD-HFRP is done to study the relative significance of the cutting speed and the feed rate.Table 1Levels of the variables used in the experiment. Process parameters Low (1) Center (2) High (3) Speed (A) in rpm 1000 1500 2000 Feed (B) in mm/min 100 200 300 3
4. International Journal of Mechanical Engineering Research and Development (IJMERD), ISSN 2248 –9347(Print) ISSN 2228 – 9355(Online), Volume 2, Number 1, January- September (2012)3. MEASUREMENT OF DELAMINATION FACTORTo determine the differing extent of intrinsic hole machining defects (delamination)caused by drilling, both the upper (Peel up delamination) and lower (Push downdelamination) surfaces of each specimens were examined using The Mitutoyo TM 500toolmakers’ microscope of 1µm resolution with 30X magnification was employed tomeasure the delamination damage of holes and each trial was replicated twice, as it canbe observed in Fig. 2. The value of delamination factor (Fd) can be obtained by thefollowing equation:Fd = Dmax / D (1)where, Dmax is the maximum diameter of the damage around the hole periphery and D isdiameter of the drill. Fig.2. Measurement of the maximum diameter (Dmax) with a tool maker’s microscope.The average readings of two trials of delamination factor were taken as process response.Table 2 presents the experimental layout plan and the computed values of delaminationfactor.Table 2Design and experimental results of the L9 orthogonal array experiment Sl. Factors Push down delamination Peel up delamination no. A B Trial 1 Trial 2 Trial 1 Trial 2 1 1 1 2.00 1.80 1.80 1.60 2 1 2 2.80 2.60 2.40 2.20 3 1 3 3.60 3.50 2.80 2.40 4 2 1 1.20 1.00 1.00 0.80 5 2 2 1.60 1.80 1.40 1.20 6 2 3 2.20 2.00 1.80 2.20 7 3 1 0.70 0.80 0.30 0.40 8 3 2 1.60 1.80 0.80 0.96 9 3 3 1.70 2.00 1.0 1.25 4
5. International Journal of Mechanical Engineering Research and Development (IJMERD), ISSN 2248 –9347(Print) ISSN 2228 – 9355(Online), Volume 2, Number 1, January- September (2012)4. EXPERIMENTAL RESULTS AND DATA ANALYSIS4.1. Analysis of S/N ratioIn the Taguchi method, the term ‘signal’ represents the desirable value (mean) for theoutput characteristic and the term ‘noise’ represents the undesirable value (S.D.) for theoutput characteristic. Therefore, the S/N ratio is the ratio of the mean to the S.D. Taguchiuses the S/N ratio to measure the quality character deviating from the desired value. TheS/N ratio η is defined asη = − 10 log10 (M.S.D.) (2)where M.S.D. is the mean-square deviation for the output characteristic.To obtain optimal cutting performance, the-lower-the-better quality characteristics fordelamination should be taken for obtaining optimal cutting performance. The optimumprocess design is achieved when the S/N ratio is maximized. Since − log is amonotonically decreasing the function, it implies that we should maximize. The M.S.D.for the-lower-the-better quality characteristic can be expressed as: 1 m 2 M .S .D. = ∑ Fi (3) M i =1 where Fi is the value of delamiantion factor for the ith test and M is the number of tests.The response obtained from experiments was analyzed using response table and graphicalrepresentation of mean effects and interaction effect of parameters on the qualitycharacteristics. Table (3) shows the experimental results for delamination factors of pushdown delamination and peel up delamination and the corresponding S/N ratio using Eqs.(2) and (3). The S/N response graph for push down and peel up delaminations are shownin Figure (3). Regardless of the-lower-the-better of the-higher-the-better qualitycharacteristic, the greater S/N ratio corresponds to the smaller variance of the outputcharacteristic around the desired value (Eqs. (2) and (3)). Therefore, based on the S/N,the optimal parameters for peel up delamination are the feed rate at level 1 (100mm/min), the cutting speed at level 3 (2000rpm). Similarly, the optimum parameters forpush down delamination are the feed rate at level 1 (100 mm/min), the cutting speed atlevel 3 (2000 rpm).Table 3Response for raw data and S/N ratios of delamination for smaller is better Push down delamination Peel up delamination factor factor Average Values Average Values Parameter Level 1 Level 2 Level 3 Level 1 Level 2 Level 3 raw Speed (A) 2.717 1.633 1.433 2.200 1.400 0.785 data Feed (B) 1.250 2.033 2.500 0.983 1.493 1.908 S/N Speed (A) -8.409 -3.981 -2.505 -6.731 -2.502 3.01 data Feed (B) -1.324 -5.960 -7.611 1.756 -2.824 -5.155 5
6. International Journal of Mechanical Engineering Research and Development (IJMERD), ISSN 2248 –9347(Print) ISSN 2228 – 9355(Online), Volume 2, Number 1, January- September (2012) Main Effects Plot for SN ratios (Push down delamination) Main Effects Plot for SN ratios (Peel up delamination) Data Means Data Means Speed Feed Speed Feed -1 4 -2 2 -3 Mean of SN ratios Mean of SN ratios 0 -4 -5 -2 -6 -4 -7 -6 -8 -9 -8 1 2 3 1 2 3 1 2 3 1 2 3 Signal-to-noise: Smaller is better Signal-to-noise: Smaller is better Fig. 3. Push down and Peel up delamination main effect plots for S/N ratio.4.2. Analysis of variance:The purpose of the analysis of variance (ANOVA) is to investigate the design parameterssignificantly affect the quality characteristic of a product or process. This is accomplishedby separating the total variability of the S/N ratios, which is measured by the sum of thesquared deviations from the total mean S/N ratio, into contributions by each of the designparameters. Statistically, there is a tool called an F test named after Fisher to see whichdesign parameters has a significant effect on the quality characteristic. In performing theF test, the mean of squared deviations due to each design parameter needs to becalculated. Then, the F value for each design parameter is simply the ratio of the mean ofsquared deviations to the mean of squared error. Usually, when F > 4, it means that thechange of the design parameter has a significant effect on the quality characteristic.From Table 4, which gives ANOVA response results, it can be found that cutting speedand feed rate are the significant parameters affecting the peel up delamination and feedrate and cutting speed are the significant parameters affecting the push downdelamination. Figure (4) illustrate the interaction plots for different S/N ratios for pushdown and peel delaminations.Table 4ANOVA response for push down and Peel up delaminationa Push down delamination Peel up delamination Seq Adj Seq Adj Source DF SS MS F P SS MS F P Speed 2 56.63 28.315 23.53 0.006 143.13 71.56 20.75 0.008 Feed 2 63.74 31.873 26.49 0.005 74.18 37.09 10.75 0.025 Error 4 4.813 1.203 13.8 3.45 Total 8a Using adjusted SS for tests. 6
7. International Journal of Mechanical Engineering Research and Development (IJMERD), ISSN 2248 –9347(Print) ISSN 2228 – 9355(Online), Volume 2, Number 1, January- September (2012) Interaction Plot for SN ratios (Push down delamination) Interaction Plot for SN ratios (Peel up delamination) Data Means Data Means 1 2 3 1 2 3 10 Speed Speed 0 1 1 2 5 2 3 3 -4 0 Speed Speed -8 -5 -12 10 -10 Feed Feed 0 1 1 2 5 2 3 3 -4 0 Feed Feed -8 -5 -12 -10 1 2 3 1 2 3 Signal-to-noise: Smaller is better Signal-to-noise: Smaller is better Fig. 4. Push down and Peel up delamination interaction plots for S/N ratios.5. CONCLUSIONSFrom the analysis of results in drilling of HFRP composite plates using conceptual S/Nratio approach, ANOVA and response surfaces, the following can be concluded from thepresent study within the range of the experiments.(1) As seen in this study, the Taguchi method provides a systematic and efficientmethodology for the design optimization of the process parameters resulting in theminimum delamination with far less effect than would be required for most optimizationtechniques.(2) Based on the S/N, the optimal parameters for the minimum peel up delamination arethe feed rate at level 1 (100 mm/min), the cutting speed at level 3 (2000 rpm).(3) Similarly, the optimum parameters for the minimum push down delamination are thefeed rate at level 1 (100 mm/min), the cutting speed at level 3 (2000 rpm).(4) The feed rate and cutting parameters influences the push down and peel updelaminations. Therefore, the feed rate and cutting speed seems to be the most criticalparameters and should be selected carefully in order to reduce all kinds of damages.(5) Conceptual S/N ratio and ANOVA approaches for data analysis draw similarconclusion.REFERENCES1. Jain S, Kumar R, Jindal UC. Mechanical behavior of bamboo and bamboo composite. J Mater Sci 1992; 27:4598–604.2. Varghese S, Kuriakose B, Thomas S. Stress relaxation in short sisal-fibre reinforced natural rubber composites. J Appl Polym Sci 1994; 53:1051–60.3. Geethamma VG, Joseph R, Thomas S. Short coir fibre-reinforced natural rubber composites: effects of fibre length, orientation and alkali treatment. J App Polym Sci 1995;55:583–94.4. Ahlblad G, Kron A, Stenberg B. Effects of plasma treatment on mechanical properties of rubber/cellulose fibre composites. Polym Int 1994; 33:103–9.5. Li Y, Mai Y-W, Lin Y. Sisal fibre and its composites: a review of recent developments. Compos Sci Technol 2000; 60:2037–55. 7
8. International Journal of Mechanical Engineering Research and Development (IJMERD), ISSN 2248 –9347(Print) ISSN 2228 – 9355(Online), Volume 2, Number 1, January- September (2012)6. Koenig W, Wulf C, Grass P, Willerscheid H. Machining of fiber reinforced plastics. Manufact Tech CIRP Ann 1985; 34(2):537–48.7. Miller JA. Drilling graphite/epoxy at Lockheed. Am Mach Autom Manufact 1987; 70–1.8. Chambers A, Bishop G. The drilling of carbon fibre polymer matrix composites. Process Manufact 1995; III, 565–72.9. Lin SC, Chen IK. Drilling of carbon fiber-reinforced composite material at high speed. Int J Mac Tools Manufact 1996; 156–62.10. Chen W. Some experimental investigations in the drilling of carbon fibre-reinforced plastic (CFRP) composite laminates. Int J Mach Tools Manufact 1997; 37(8):1097– 108.11. Piquet R, Ferret B, Lachaud F, Swider P. Experimental analysis of drilling damage in thin carbon/epoxy laminate using special drills. Int J Mac Tools Manufact 2000; 1107–15.12. Ugo Enemuoh E, Sherif El-Gizawy A, Chukwujekwu Okafor A. An approach for development of damage-free drilling of carbon fiber reinforced thermosets. Int J Mac Tools Manufact 2001; 1795–814. 8
Be the first to comment